# Dynamic multi-axial behavior of shape memory alloy nanowires with coupled thermo-mechanical phase-field models

Post on 24-Jan-2017

217 views

TRANSCRIPT

Dynamic multi-axial behavior of shape memory alloynanowires with coupled thermo-mechanical phase-fieldmodels

R. P. Dhote R. N. V. Melnik J. Zu

Received: 13 July 2013 / Accepted: 22 March 2014

The Author(s) 2014

Abstract The objective of this paper is to provide

new insight into the dynamic thermo-mechanical

properties of shape memory alloy (SMA) nanowires

subjected to multi-axial loadings. The phase-field

model with GinzburgLandau energy, having appro-

priate strain based order parameter and strain gradient

energy contributions, is used to study the martensitic

transformations in the representative 2D square-to-

rectangular phase transformations for FePd SMA

nanowires. The microstructure and mechanical behav-

ior of martensitic transformations in SMA nanostruc-

tures have been studied extensively in the literature for

uniaxial loading, usually under isothermal assump-

tions. The developed model describes the martensitic

transformations in SMAs based on the equations for

momentum and energy with bi-directional coupling

via strain, strain rate and temperature. These govern-

ing equations of the thermo-mechanical model are

numerically solved simultaneously for different

external loadings starting with the evolved twinned

and austenitic phases. We observed a strong influence

of multi-axial loading on dynamic thermo-mechanical

properties of SMA nanowires. Notably, the multi-axial

loadings are quite distinct as compared to the uniaxial

loading case, and the particular axial stress level is

reached at a lower strain. The SMA behaviors

predicted by the model are in qualitative agreements

with experimental and numerical results published in

the literature. The new results reported here on the

nanowire response to multi-axial loadings provide

new physical insight into underlying phenomena and

are important, for example, in developing better SMA-

based MEMS and NEMS devices

Keywords Shape memory alloy Thermo-mechanical coupling Multi-axial loading Phase-field model Nanowire

1 Introduction

The unique shape recovering characteristics, high

energy density, and high actuation strain of shape

memory alloys (SMAs) make them ideal candidates

for use in macro-, micro-, and nano- scale actuators,

sensors and transducers [16]. The shape recovering

characteristics give rise to the complex nonlinear

mechanical behavior of these materials. The com-

plexity arises because of the coupling between thermal

R. P. Dhote (&) J. ZuMechanical and Industrial Engineering, University of

Toronto, 5 Kings College Road, Toronto, ON M5S-3G8,

Canada

e-mail: rakesh.dhote@mail.utoronto.ca

R. P. Dhote R. N. V. MelnikM2NeT Laboratory, Wilfrid Laurier University, 75

University Avenue, Waterloo, ON N2L-3C5, Canada

R. N. V. Melnik

Universidad Carlos III de Madrid, Avenida de la

Universidad 30, E28911 Leganes, Spain

123

Meccanica

DOI 10.1007/s11012-014-9938-5

and mechanical (or structural) physics, and due to

martensitic transformations (MTs)

SMAs have been extensively studied (see e.g., [7

11]) and used in commercial applications [10, 1216].

Most of the applications to date are designed to exploit

the uniaxial properties of SMA wires, and there is a

vast literature on experimental data of ubiquitous

uniaxial tensile tests. However, in many of the

applications in fields such as bioengineering and

nanotechnology, SMA specimens are often subjected

to multi-axial loadings [14, 1719]. For such advanced

applications, further knowledge of multi-axial prop-

erties of SMAs is required, yet very few experimental

data on multi-axial response of SMA specimens are

available in the literature [2026]. Tokuda et al. [20]

and Sittner et al. [21] conducted combined tension-

torsion experiments on thin wall Cu- based polycrys-

talline SMA specimens and reported a coupling

between tension and torsion during forward and

reverse transformations that can be used to control

the axial strain via torque and vice versa. The variation

in mechanical properties subjected to multi-axial

loadings has been experimentally confirmed by Lim

and McDowell [22], and Bouvet et al. [23]. McNaney

et al. [24] investigated variations in mechanical

responses during biaxial tension-torsion experiments

on NiTi thin wall tubes subjected to various loading

and unloading paths under isothermal conditions.

Recently, Lavernhe-Taillard et al. [25] and Grabe

and Bruhns [26] conducted several multi-axial ten-

sion-torsion experiments on thin wall NiTi tubes

which showed significant differences in mechanical

behavior of SMAs. The above studies suggested that

the variation in mechanical response stems from the

nucleation of energetically favorable martensitic

variants to applied loadings. However, most of the

above studies focused on experimental stressstrain

curves with little focus on underlying MTs.

The controlled experiments in SMAs are complex

because of required simultaneous control of stress and

deformation in time and space. In addition, the multi-

axial experimental setups are expensive and time

consuming. Hence, models have been developed to

predict the properties of SMA structures for design and

optimization. Several modeling approaches have been

developed to predict the SMA properties. The majority

of the models in the literature focused on uniaxial

tensile test data. Extensive reviews of such models for

SMAs have been discussed in [810, 2729]. With the

need of predicting multi-axial properties of SMAs for

advanced technological applications, there has been an

increasing focus on the development of multi-axial

models [3035]. Tokuda et al. [30] proposed a two

dimensional micromechanical model based on crystal

plasticity and the deformation gradient to describe

thermo-mechanical behavior in polycrystalline Cu-

based SMAs subjected to multi-axial loadings. Bouvet

et al. [31] presented a phenomenological model taking

into account tension-compression asymmetry for pre-

dicting pseudoelastic behavior of SMAs under multi-

axial loadings using two phase transformations sur-

faces. Thiebaud et al. [32] used a phenomenological

model developed by Raniecki et al. [36] to simulate

internal loops in order to characterize the stiffness and

the damping effect by an equivalent complex Youngs

modulus approach under static strain offsets. A rate-

independent crystal mechanics based model developed

by Pan et al. [33] is used to quantitatively predict the

experimental response of the NiTi rod under tension

torsion loading conditions. Arghavani et al. [34]

presented a phenomenological model, based on the

framework of irreversible thermodynamics, that uses

stress-induced martensite as scalar internal variable

and the preferred direction of the variants as indepen-

dent tensorial internal variable to predict the experi-

mentally observed SMA behavior subjected to multi-

axial loadings. Recently, Saleeb et al. [35] proposed a

fully general three dimensional SMA model, based on

partitioning of the stored and dissipated mechanical

energies by utilizing the notion of multiplicity of

inelastic mechanisms, to capture numerous uniaxial

and multi-axial experimental responses of SMA

material. All the above studies indicate the importance

of multi-axial loadings on the SMA properties.

We are interested here specifically in the phase-

field (PF) models that have emerged as a powerful

computational approach for modeling microstructures

and mechanical properties of solid-to-solid phase

transformations in SMAs [3747]. This approach

provides a unified framework that allows to describe

stress and temperature induced phase transformations,

including their dynamics in the variational setting. The

PF models have been used to study microstructure and

mechanical properties of meso- and nano-scale SMA

specimens. Bouville and Ahluwalia [45] used the PF

model with the GinzburgLandau free energy to study

the microstructure in constrained nanostructures and

mechanical properties of infinite length nanowires

Meccanica

123

subjected to axial loading. They observed size depen-

dent properties and size effects in nanostructures.

Ahluwalia et al. [43] carried out the three dimensional

simulations to study the axial properties of nanosize

samples with periodic boundary conditions for the

cubic-to-tetragonal phase transformations in the FePd

crystals. They investigated changes in the stressstrain

behavior as a function of strain rate. Idesman et al. [48]

studied the evolution of microstructures in periodic

nanosized three dimensional NiAl samples using the

advanced potential developed by Levitas and Preston

[42]. Although SMAs possess strong temperature

dependent properties [10], most of the above studies

were carried out under the assumption of isothermal

conditions. In the series of papers by Melnik and

coworkers [38, 39, 4953] a coupled thermo-mechan-

ical PF models have been used to study the dynamics

of SMAs based on the GinzburgLandau free energy.

Nevertheless, most of the studies focused on the

mechanical behavior of SMA structures under uniaxial

loadings only. However, as mentioned above, impor-

tant applications exist where the SMA structure may

induce multi-axial loading during interactions with its

environment.

In this paper, the objective is to study the properties

of finite length nanowires with a fully coupled non-

linear thermo-mechanical formulation under multi-

axial loadings. We use the mesoscale PF model

developed in our earlier work [54, 55] to study the

SMA dynamics based on the GinzburgLandau free

energy of 2D square-to-rectangular phase transforma-

tions. The details of size dependent properties and size

effects in SMA nanostructures using the developed

coupled thermo-mechanical model have been dis-

cussed in Dhote et al. [53]. In Dhote et al. [56], we

performed the first fully coupled thermo-mechanical

multi-axial loadings experiments on finite length SMA

nanowires using the PF model in the dynamic setting

and presented preliminary studies on the behavior of

SMA nanowire initially in twinned microstructure.

Here, we carry out a detailed study and conduct series

of complex multi-axial numerical experiments to

understand the microstructure evolution and its impact

on stressstrain properties of SMA nanowires initially

in twinned and austenite phases.

The rest of the paper is organized as follows. In

Sect. 2, we present a general mathematical framework

for modeling the SMA dynamics for 2D square-to-

rectangular phase transformations. We conduct a

series of numerical experiments with different multi-

axial loading conditions on SMA nanowires. In Sect.

3, we investigate the effect of microstructure on the

thermo-mechanical behavior of SMAs upon multi-

axial loadings. Finally, Sect. 4 summarizes the results

and discusses the scope for future work.

2 SMA dynamics

The mathematical model to study the SMA dynamics

is based on a mesoscale model analyzed in detail

numerically in our earlier works [53, 55]. In this work,

our focus is on the thermo-mechanical behavior of

FePd nanowires subjected to multi-axial loadings

based on microstructure evolution. The FePd material

has a high temperature, high-symmetry face centered

cubic (FCC) austenite phase, as well as low temper-

ature, low-symmetry face-centered tetragonal (FCT)

martensitic phases (with tetragonal crystal aligned

with elongated side along three rectilinear directions).

The material exhibits cubic-to-tetragonal martensitic

phase transformations under thermal and mechanical

loadings. The martensitic phase transformation is a

highly nonlinear phenomenon. In addition, the cou-

pled thermo-mechanical model and three dimensional

simulations make computations challenging [39, 50].

To make the computation tractable, we study the

MTs using the simplified 2D square-to-rectangular

representative phase transformations under the

assumption that the deformation in the out-of-plane

direction is constant. The effect of the third direction

deformation on microstructure evolution has been

reported elsewhere with the 3D dynamic thermo-

mechanical phase-field models [57, 58]. However,

here we focus on the 2D square-to-rectangular phase

transformations in SMAs, where the square represents

the austenite phase A and the rectangles represent the

martensitic variants M and M (with rectanglelength aligned along two perpendicular axes). As the

austenite and martensite variants have different ener-

gies and prevail at different temperatures, the phase

transformations in SMA can be modeled by using the

GinzburgLandau free energy [52, 54].

As per Falk [59], strains in the domain can be used

to describe different phases in the domain. The strain

components which directly contribute to PT are called

order-parameters (ops), and the others are called non-

OPs (nop). For square-to-rectangular PT, the

Meccanica

123

deviatoric strain e2 serves as an OP. The free energyF

of PT is described as

F Fop Fnop Fgradient; 1

where Fop is the energy part due to the OPs, which

contributes to MT as per the LandauDevonshire

theory, Fnop is the energy part due to non-OPs, which

contributes to the bulk and shear energy, and Fgradientis the energy part which contributes to the energy cost

required to maintain different domain phases in a

domain and interface formed between physical bound-

aries and domain. The gradient energy term (or the

Ginzburg energy) maintains a non-zero width in

austenite-martensite and martensite-martensite inter-

faces, and prevents the system from creating an

infinite number of interfaces (e.g. [60]). The gradient

term introduces a nano length scale width of a domain

wall in the model ([41, 43] and references within). As a

result, the LandauGinzburg theory has been applied

to nanoferroelastic and nanoferroelectric systems to

study the dynamic behavior of nanostructures [45, 61].

The free energy components in (1) for 2D square-

to-rectangular PTs are defined as

Fop a2

2

h hmhm

e22

a4

4e42

a6

6e62;

Fnop a1

2e21

a3

2e23;

Fgradient kg

2

oe2

ox1

2 oe2

ox2

2" #;

2

where e1; e2 and e3 are the hydrostatic, deviatoric and

shear strain respectively defined as e1 xx yy

=ffiffiffi2

p; e2 xx yy

=

ffiffiffi2

p; e3 xy yx

=2; with

ij oui=oxj

ouj=oxi

=2 being the Cauchy

Lagrange infinitesimal strain tensor; ui; i 1; 2 aredisplacements along x1 and x2 directions, respectively

(refer to Fig. 2) , h is the material temperature, hm is theaustenite-martensite phase transformation tempera-

ture, ai are the material constants, and kg is the

Ginzburg coefficient. As the maximum strain induced

in the domain is 3 % (refer to Table 1), a geometriclinear kinematic (infinitesimal) relationship is a simple

and convenient assumption. The influence of large

strain (geometric non-linear) definition (large strain

and material rotation) in the model and its effect on the

phase transformations, due to finite rotation, have been

highlighted by Clayton and Knap [62], Hildebrand and

Miehe [63], Levin et al. [64] and in references [65, 66].

As discussed above, the deviatoric strain e2 is

selected as the order parameter to distinguish different

phases in a domain. The austenite phase exists when

strains in both directions are equal i.e. e2 0(ou1=ox1 ou2=ox2). The martensite variants Mexist when the strain in x1 direction is greater than

strain in x2 direction i.e. e2 [ 0 (ou1=ox1 [ ou2=ox2),and the martensite variant M exist when the strain inx2 direction is greater than strain in x1 direction i.e.

e2\0 (ou1=ox1\ou2=ox2). With the free energygiven by (1), the SMA behavior is captured by the

mathematical model that couples the structural and

thermal fields using the conservation equations of

mass, momentum, and energy in the way described

previously in Melnik et al. [49].

The governing equations of SMA dynamics are

obtained by minimizing the total energy in a domain.

The kinetic energy K, and the dissipation functional

R are given by

Kt q2

v2i ; and Rui; t g2

_u2i;j; 3

where q is the mass density, g is the dissipationcoefficient, vi _ui is the velocity in the ith direction,and _ui;j refers to the differentiation of velocity ui in j

direction, with i; j 1; 2 respectively.The Lagrangian L and the Hamiltonian H of the

system are defined as

L Kt FRui; t; 4

H Z t

0

ZX

L fiui dXdt; 5

where fi are the mechanical loadings in the ith

direction, X is the SMA domain, and 0; t is the timespan.

Table 1 Numerical experimentsmulti-axial loading patterns

Set

no.

Expt.

no.

Axial Bending

va% tsa(ns)

tla(ns)

vb% tsb(ns)

tlb(ns)

I 1 3 0 1 0 0 0

2 0 0 0 3 0 1

3 3 0 1 3 0 1

II 4 3 0 1 3 1/8 1/6

5 3 0 1 3 1/5 1/4

6 3 0 1 3/2 1/5 1/4

Meccanica

123

Using the Hamiltonian principle, the structural (or

mechanical) dynamics equations are obtained as

qo2ui

ot2

X orijoxj

rgi gr2vi fi; 6

where rij o=oij Fop Fnop

, and rgi o=oijFg [53]. On simplification, we obtain the stresstensor components as

r11 1ffiffiffi2

p a1e1 a2h hm

hm

e2 a4e32 a6e52

;

7

r12 1

2a3e3; 8

r21 r12; 9

r22 1ffiffiffi2

p a1e1 a2h hm

hm

e2 a4e32 a6e52

;

10

and the rgi components are

rg1 kg o4u1

ox41 o

4u1

ox21ox22

o4u2

ox31ox2 o

4u2

ox1ox32

;

11

rg2 kgo4u1

ox31ox2 o

4u1

ox1ox32

o4u2

ox21ox22

o4u2

ox42

: 12

Equations (710) define the material behavior in

square-to-rectangular PTs. The fourth order terms in

(1112) are the extra stress terms which correspond to

the strain gradient terms in the free energy F, and

represent the domain walls between different phases

of the martensites.

The governing equation of the thermal field is

obtained by the conservation laws of internal energy

[49] as

qoe

ot rT : rv r q g; 13

where q jrh is the Fourier heat flux vector (asmentioned in Melnik et al. [39], the hyperbolic

Cattaneo-Vernotte law may be more appropriate in

some cases), j is the heat conductance coefficient ofthe material, and g is the thermal loading. The internal

energy is connected with the potential energy con-

structed above via the Helmholtz free energy W as

e Wh; e h oWh; eoh

;

Wh; e F Cvhlnh;14

where Cv is the specific heat of a material.

On substituting (14) in the (13), the governing

equation of the thermal field in two dimensions can be

given as

qCvohot

j o2hox2

o2hoy2

a2

hhm

e2oe2

ot g: 15

The second term on the right hand side of (15) is a

non-linear term, which couples temperature, defor-

mation gradient (strain), and rate of deformation

gradient (strain rate). Hence the overall system of

(6) and (15) describes the non-linear thermo-

mechanical coupled behavior of SMAs via h; e2,and _e2.

In Dhote et al. [53], we used (6) and (15) to study

the behavior of SMA nanostructures of different

sizes. We also captured the martensitic transforma-

tion suppression phenomenon and size dependent

properties observed experimentally and numerically

(see e.g., [45, 67]) by using the developed thermo-

mechanical model. We also conducted the uniaxial

loadings on the nanowire under the assumption of

isothermal conditions. The results were in qualita-

tive agreement with the results obtained from

uncoupled models (e.g. [45]). We also obtained

qualitative agreement in temperature evolution dur-

ing dynamic loading and unloading of the SMA

specimen with the experimental work conducted by

Gadaj et al. [68] and Pieczyska et al. [69, 70] using

the developed thermo-mechanical model. In Dhote

et al. [56], we carried out the preliminary studies of

nanowire behavior subjected to multi-axial loadings

with nanowire initially in twinned martensitic phase.

We extend the study here with additional complex

multi-axial loading experiments starting with nano-

wire initially in twinned phase and a new set of

simulations starting with nanowire in austenite

phase. In the remainder of this paper, we focus on

the results of numerical simulations of SMA nano-

wires subjected to multi-axial loadings. Before we

proceed, we remark that currently our model does

not account explicitly for surface effects [71],

however the developed framework can be easily

extended to incorporate them.

Meccanica

123

3 Numerical simulations

The Eqs. (6) and (15) are rescaled in the spatio-

temporal domain for numerical convenience and

solved numerically using the finite element method.

We have implemented the equations in the Comsol

Multi-physics software [72] by first splitting the fourth

order differential terms into two second order differ-

ential terms. As the experimental studies of dynamic

multi-axial behaviors in SMA nanowires are not

available in the literature, we validate the model at

different stages as described in the following sections.

We first verify the developed model and its numerical

implementation using a test problem [73]. A unit

square plate insulated and constrained in the normal

directions on the three edges, and subjected to sudden

unit heating on the fourth edge as schematically

depicted in Fig. 1a. We reduce the system of (6) and

(15) to the homogeneous thermo-elastic equations [74]

under the following assumptions:

the unit square plate is in plane strain condition,

the higher power strain terms a4 and a6, account-

ing for the phase transformations, are neglected,

the phase transformation is homogeneous i.e. the

Ginzburg term kg is neglected, and

(a)

(c) (d)

(b)

Fig. 1 Comparison of dimensionless numerical and analytical results [73] for a test problem on a unit square plate

Meccanica

123

the second term on the right hand side of (15) is

neglected.

The resulting equations are solved numerically, as

mentioned above, and the dimensionless results are

compared with the analytical solutions in Park and

Banerjee [73]. The dimensionless temperature h, stressr11, and displacement u2 profiles at the points A, B,and C, respectively in Fig. 1 are in agreement with the

analytical homogeneous solutions of thermo-elastic-

ity. We also solved the non-homogeneous system of

equations with dynamic thermo-mechanical coupling.

The results are in qualitative agreement with exper-

imental and numerical results as described in detail in

the subsequent sections.

Next, we perform the numerical experiments on

rectangular domain (X) nanowires of dimension1000 200 nm with sides parallel to 10h i and 01h idirections defined with reference to the austenite phase

as shown in Fig. 2a. The FePd material parameters

used for the simulations are (see e.g., [45]):

a1 140 GPa, a3 280 GPa, a2 212 GPa, a4 17 103 GPa, a6 30 106 GPa, hm 265 K, g 0:025 Nsm2, kg 3:5 108 N, Cv 350 Jkg1K1, and j 78 Wm1K1.

3.1 Microstructure evolution

The series of numerical simulations have been

conducted to study the response of the nanowire to

multi-axial loadings. The nanowires are subjected to

different temperatures hinit for sufficiently long time toevolve into the twinned [56] and austenite phases. The

strategy adopted here is to first evolve the

microstructure in the domain and then use the evolved

microstructure as an initial condition in the multi-axial

loading simulations.

The boundary and initial conditions used during

microstructure evolutions are

uijoX;t 0; rui njoX;t 0; rh njoX;t 0;hjX;t0 hinitK; uijX;t0 white noise; 16

where n is the normal vector to the boundary. During

microstructure evolution, the mechanical boundary

conditions are set to u = 0 on all the boundaries. All the

simulations in the paper have been conducted under

the assumption of adiabatic temperature conditions on

all the boundaries. The simulations have been per-

formed on the finite domain size with constrained or

stress-free boundary conditions. The nanowire is set to

the initial temperature hinit 250K; and 270 K toevolve into the twinned, and austenite phases

respectively.

The microstructures are allowed to evolve till it gets

stabilized over a long simulation time. The evolved

microstructures is shown in Fig. 3. The red and blue

colors represent the M and M martensitic variantsand the green color represents the A phase. Figure 3a

shows the evolved twinned martensite phase, and Fig.

3b shows the evolved austenite phase. The evolved

microstructure in twinned martensite is self-accom-

modated and forms domain walls oriented in f11g orf11g planes to minimize the energy [7577]. Duringthe microstructure evolution, the temperature increase

is observed due to the insulated boundary conditions

and thermo-mechanical coupling between tempera-

ture h, strain e2, and strain rate _e2.

(a) (b)

Fig. 2 Schematic indicating a direction, plane, and boundary (oX) nomenclature in the nanowire domain (X) and loadings duringmulti-axial loadings [56], and b displacement based ramp loading and unloading

Meccanica

123

3.2 Multi-axial loading

We now perform the multi-axial loading simulations

on the evolved microstructure from the previous

subsection. We consider the evolved microstructure

as an initial condition to the loading experiments. In

order to investigate the response of the nanowire to

different loading patterns, we carried out a series of

numerical experiments as described in Table 1. The

simple experiments with axial (experiment 1) and

bending (experiment 2) loads have been first con-

ducted and the response of nanowire has been

compared with multi-axial loadings (experiment 3,

i.e. axial and bending loads applied simultaneously).

Next, different patterns of multi-axial loadings have

been applied to study the nanowire response to

complex loadings. The initial and boundary conditions

for all the simulations are:

uijoX1;t 0; rui njoX;t 0; rh njoX;t 017

and the loading conditions for different loading cases

are

Axial :u1joX4;t da;Bending :u2joX4;t db;

Multi axial :u1joX4;t da; 2 joX4;t db;18

where da and db are the ramp displacement based

loading and unloading with axial va and bending vbdisplacements, respectively, as shown in Fig. 2b. The

expressions for ramp displacement based loading and

unloading are

da va tla jt tsa tlaj tla

tla tsa

;

db vb tlb jt tsb tlbj tlb

tlb tsb

;

19

where tsa and tsb are the start of loading times, tla and

tlb are the loading times to reach va and vb

displacements for axial and bending loadings respec-

tively. Next, we conducted the numerical experiments

on the evolved nanowire in twinned martensite and

austenite from the previous section.

3.2.1 Nanowire with twinned microstructure

as an initial condition

Here, we first present the results of first three

experiments in Table 1 reported in [56] for the sake

of completeness and then discuss the complex multi-

axial loading experiments carried out additionally to

understand the dynamic thermo-mechanical properties

of SMA nanowires.

The nanowire with evolved twinned microstruc-

ture, as shown in Fig. 3a, is used as an initial condition

for the multi-axial loading experiments. The nanowire

is loaded in the axial (experiment 1), bending (exper-

iment 2), and multi-axial (experiment 3) directions as

mentioned in Table 1. The simulations are performed

for each loading case individually. We presented the

results of the above three experiments in Dhote et al.

[56]. In axial loading, the twinned microstructure is

converted to a favorable martensitic phase (M) to theaxial loading via a process of detwinning, as also

reported experimentally [78]. The elastic loading and

phase transformations occur simultaneously. In the

case of bending load, the phase transformations occur

in a localized area and the redistribution of martensitic

domains has been observed. The redistribution of

martensitic domains is governed by the local axial

stress sign. The phenomenon of redistribution of

martensite has also been experimentally reported by

Rejzner et al. [79] in Cu- based SMAs subjected to

pure bending. In the multi-axial case (experiment 3),

the mixed behavior of elastic loading, detwinning, and

redistribution of martensitic domains is observed. The

simultaneous occurrence of these phenomena affects

the mechanical properties of SMA nanowires.

The microstructures evolution has been quantita-

tively studied by comparing the normalized area of

(a) (b)

Fig. 3 (Color online) Evolution of a twinned [56], and b austenite microstructure in the nanowire (red and blue indicates martensitevariants and green indicates austenite)

Meccanica

123

different phases in the domain by defining the

parameter Ah as

Ah Area of martensite or austenite phase

Area of the nanowire; 20

where h refer to M and M variants and A phase.Figure 4a shows the evolution of Ah for the three

loading cases mentioned above. The observations of

elastic loadings, phase transformations, and redistri-

bution of martensites under different loading condi-

tions has also been predicted from the Fig. 4a.

The axial stressstrain behavior of nanowires for

the axial (experiment 1) and multi-axial (experiment

3) case (refer to solid and dotted lines) is shown in Fig.

5a. In the multi-axial loading case, the shear strains are

non-zero and are coupled with the axial components of

deformation. The stressstrain characteristics of nano-

wire under multi-axial loadings are quite distinct as

compared to the uniaxial loading and the particular

stress level is reached at a lower strain. The existing

variants lead to higher stresses due to a higher energy

state of multi-axial loading. The temperature evolu-

tion for different loading cases (refer to the solid lines)

is shown in Fig. 5b. The increase and decrease of

temperature upon loading and unloading has been

verified experimentally by the works of Gadaj et al.

[68] and Pieczyska et al. [69, 70]. The temperature

increase in the bending case is not steep as compared

to the axial case because the variants are redistributed

in a domain.

The above experiments provide insight into the

response of nanowire subjected to dynamic axial,

bending, and multi-axial loadings. Further new sets of

simulations have been carried out with complex multi-

axial loading patterns to study nanowire response. The

nanowires have been subjected to different complex

multi-axial loading casesexperiments 4, 5, and 6

(refer to Table 1). These experiments refer to the

application of bending loads with different

vb; tsb ; tlb .The time-snapshots of microstructure evolu-tion for three multi-axial experiments are shown in

Fig. 6ac. It is observed that the dynamics of loading

causes the evolution of microstructures in different

patterns. The axial stressstrain curves for three

experiments are shown in Fig. 7a. A significant

difference in response of nanowires to dynamic

loadings is evident from the variation in stressstrain

curves for complex loading cases. The sudden appli-

cation of bending load causes increased (sudden jump

in) axial stiffness of the nanowire, which reduce

subsequently as the deformation wave travels and the

load is distributed in the whole domain. The combi-

nation of magnitude of vb and its loadingunloadingduration tsb ; tlb would dictate the dynamics of elastic

(a) (b)

Fig. 4 (Color online) Evolution of Ah with time starting frominitial a twinned martensite and b austenite conditions fordifferent loading cases: axial (red), bending (black), and multi-

axial (blue) (solid lines represent AM, dash lines represent

AM, and dotted line represent AA).

Meccanica

123

loading, phase transformation, and redistribution of

martesitic domains. The combined effect of these

phenomena is evident from the waviness in Ah in

Fig. 7b as compared to the microstructure evolution in

simple multi-axial experiment (experiment 3) in

Fig. 4b. The effect of complex loading characteristics

on temperature evolution dynamics is apparent from

Fig. 7c.

3.2.2 Nanowire with austenite microstructure

as an initial condition

We also conducted the numerical simulations with

nanowire in the austenite phase. The microstructure

evolution during the axial (experiment 1), bending

(experiment 2), and multi-axial (experiment 3) load-

ings are presented in Fig. 8(ac). It is observed that the

(a) (b)

Fig. 5 (Color online) Average a axial stressstrain andb temperature evolution for different loading cases: axial(red), bending (black), and multi-axial (blue) for nanowire

initially in a twinned phase (solid lines) [56], and b austenitephase (dashed line). The dotted line in a represents unloading ofthe twinned phase

(a) (b) (c)

Fig. 6 (Color online) Evolution of microstructure in the(twinned phase) nanowire subjected to multi-axial loading and

unloading in a experiment 4, b experiment 5, and c experiment 6

at time (ns) (i) 0.25, (ii) 0.375, (iii) 0.5, (iv) 1.0, (v) 1.5, and (vi)

2.0 (red and blue indicate martensite variants and green

indicates austenite)

Meccanica

123

nanowire in austenite phase is transformed into the

favorable martensite upon loadings. This transforma-

tion from austenite phase to favorable martensites, via

a movement of the habit plane in a nanowire domain,

is different from the detwinning transformation

described in Sect. 3.2.1. The movement of habit plane

is also interpreted from phase change from AA ! AMwith traces of AM during loading as shown in Fig. 4b.

An important note to make here is that the AA has

significant presence in the domain at the end of

unloading. The axial stressstrain behavior of nano-

wire for axial and multi-axial experiments are shown

in the Fig. 5a (refer to the dashed lines). The stiffness

of the nanowire in austenite phase is greater than in the

twinned martensite phase, which is also experimen-

tally observed in SMAs [10, 12]. The stressstrain

characteristics of nanowire upon multi-axial loadings

are also quite distinct than in the case of the uniaxial

loading, and the particular stress level is reached at a

lower strain. The evolution of temperature in the

nanowire is shown in Fig. 5a (refer to the dashed

lines). The microstructure evolution is in qualitative

agreement with the axial and bending loading exper-

iments on the NiTi tube [80].

Further, we carried out multi-axial loadings on

SMA nanowires with different loading conditions

described in experiments 46 in Table 1. The time

snapshots of microstructure evolution are presented in

Fig. 9. The evolution of microstructure distribution Ahindicate the dynamics of phase transformations due to

complex loadings, as shown in Fig. 10b, and its effect

on the evolution of axial stressstrain behavior, and

(a) (b) (c)

Fig. 7 (Color online) Evolution of a average axial stressstrain and b Ah, and c temperature over time for experiment 4 (red), 5 (black),and 6 (blue) for nanowire initially in the twinned phase

(a) (b) (c)

Fig. 8 (Color online) Evolution of microstructure in the(austenite phase) nanowire subjected to a axial (experiment1), b bending (experiment 2), and c multi-axial (experiment 3)

loading and unloading at time (ns) (i) 0.25, (ii) 0.5, (iii) 1.0, (iv)

1.5, and (v) 2.0 (red and blue indicate martensite variants and

green indicates austenite)

Meccanica

123

temperature as shown in Fig. 10a, c, respectively. A

strong influence of complex multi-axial loading is

observed on the dynamics of elastic loading, phase

transformation, and redistribution of martesitic

domains in SMA nanowire domains. The complex

multi-axial loading induces complex thermo-mechan-

ical behaviors in SMA nanowire.

4 Conclusions

We analyzed in detail the thermo-mechanical behavior

of FePd nanowires under complex multi-axial loading

conditions. The phase-field model with the Ginzburg

Landau free energy was used to model the square-to-

rectangular phase transformations. The simulations

were carried out accounting for the coupled thermo-

mechanical physics. The numerical results revealed

that the axial loading is dominated by the detwinning

phase transformation, while the bending case by the

redistribution of martensitic variants based on the

local axial stress sign. The multi-axial behavior of

nanowires is quite distinct as compared to the uniaxial

loading due to the combined dynamics of elastic

loading, phase transformations, and redistribution of

the martensitic variants, with particular stress reaching

at a lower strain. The multi-axial loading character-

istics causes complex thermo-mechanical behavior of

SMA nanostructures. The results of multi-axial

behaviors are important in developing better SMA

(a) (b) (c)

Fig. 9 (Color online) Evolution of microstructure in the(austenite phase) nanowire subjected to multi-axial loading

and unloading in a experiment 4, b experiment 5, and

c experiment 6 at time (ns) (i) 0.25, (ii) 0.375, (iii) 0.5, (iv)1.0, (v) 1.5, and (vi) 2.0 (red and blue indicate martensite

variants and green indicates austenite)

(a) (b) (c)

Fig. 10 (Color online) Evolution of a average axial stressstrain and b Ah, and c temperature over time for experiment 4 (red), 5(black), and experiment 6 (blue) for nanowire initially in the austenite phase

Meccanica

123

nanowire based actuators, sensors, as well as in control

of MEMS and NEMS devices.

Although the simulations enhanced our understand-

ing of microstructure evolution and its effect on

response of the material subjected to dynamic multi-

axial loading, there are current limitations in the

temporal domain due to model rescaling. Further

studies with different boundary conditions and 3D

models [81] will provide further insight into the

nanowire response to multi-axial loading dynamics.

Acknowledgments RPD, JZ and RNVM were supported byNSERC and CRC program, Canada. RM thanks colleagues at

Mevlana University for their hospitality during his visit there

and TUBITAK for its support.

References

1. Shu S, Lagoudas D, Hughes D, Wen J (1997) Modeling of a

flexible beam actuated by shape memory alloy wires. Smart

Mater Struct 6:265

2. Kahn H, Huff M, Heuer A (1998) The TiNi shape-memory

alloy and its applications for MEMS. J Micromech Micro-

eng 8:213

3. Fu Y, Du H, Huang W, Zhang S, Hu M (2004) TiNi-based

thin films in MEMS applications: a review. Sens Actuators

A 112(2):395408

4. Juan J, No M, Schuh C (2009) Nanoscale shape-memory

alloys for ultrahigh mechanical damping. Nature Nano-

technol 4(7):415419

5. Barcikowski S, Hahn A, Guggenheim M, Reimers K, Osten-

dorf A (2010) Biocompatibility of nanoactuators: stem cell

growth on laser-generated NickelTitanium shape memory

alloy nanoparticles. J Nanopart Res 12(5):17331742

6. Bayer BC, Sanjabi S, Baehtz C, Wirth CT, Esconjauregui S,

Weatherup RS, Barber ZH, Hofmann S, Robertson J (2011)

Carbon nanotube forest growth on NiTi shape memory alloy thin

films for thermal actuation.Thin SolidFilms519(18):61266129

7. Bhattacharya K (2003) Microstructure of martensite: why it

forms and how it gives rise to the shape-memory effect.

Oxford University Press, Qxford

8. Smith R (2005) Smart material systems: model development,

vol 32. Society for Industrial Mathematics, Philadelphia

9. Lagoudas D, Brinson L, Patoor E (2006) Shape memory alloys,

part II: modeling of polycrystals. Mech Mater 38(56):430462

10. Lagoudas D (2008) Shape memory alloys: modeling and

engineering applications. Springer, London

11. Yoneyama T, Miyazaki S (2008) Shape memory alloys for

biomedical applications. Woodhead Publishing

12. Otsuka K, Wayman C (1998) Shape memory materials.

Cambridge University Press, New York

13. Kohl M (2004) Shape memory microactuators. Springer,

Berlin

14. Miyazaki S, Fu Y, Huang W (2009) Thin film shape

memory alloys: fundamentals and device applications.

Cambridge University Press, Cambridge

15. Ozbulut O, Hurlebaus S, DesRoches R (2011) Seismic

response control using shape memory alloys: a review.

J Intell Mater Syst Struct 22(14):15311549

16. Elahinia M, Hashemi M, Tabesh M, Bhaduri S (2011)

Manufacturing and processing of NiTi implants: a review.

Prog Mater Sci

17. Fang D, Lu W, Hwang K (1998) Pseudoelastic behavior of

CuAINi single crystal under biaxial loading. Met Mater Int

4(4):702706

18. Shan Y, Dodson J, Abraham S, Speich JE, Rao R, Leang KK

(2007) A biaxial shape memory alloy actuated cell/tissue

stretching system. In: ASME 2007 international mechanical

engineering congress and exposition, American Society of

Mechanical Engineers, pp. 161169.

19. Niendorf T, Lackmann J, Gorny B (2011) H. Maier, Scr

Mater, In-situ characterization of martensite variant for-

mation in Nickel-Titanium shape memory alloy under

biaxial loading. Scripta Materialia

20. Tokuda M, Petr S, Takakura M, Ye M (1995) Experimental

study on performances in Cu-based shape memory alloy

under multi-axial loading conditions. Mater Sci Res Int

1(4):260265

21. Sittner P, Hara Y, Tokuda M (1995) Experimental study on

the thermoelastic martensitic transformation in shape

memory alloy polycrystal induced by combined external

forces. Metall Mater Trans A 26(11):29232935

22. Lim T, McDowell D (1999) Mechanical behavior of an Ni-

Ti shape memory alloy under axial-torsional proportional

and nonproportional loading. J Eng Mater Technol 121:9

23. Bouvet C, Calloch S, Lexcellent C (2002) Mechanical

behavior of a CuAlBe shape memory alloy under multi-

axial proportional and nonproportional loadings. J Eng

Mater Technol 124:112

24. McNaney J, Imbeni V, Jung Y, Papadopoulos P, Ritchie R

(2003) An experimental study of the superelastic effect in a

shape-memory Nitinol alloy under biaxial loading. Mech

Mater 35(10):969986

25. Lavernhe-Taillard K, Calloch S, Arbab-Chirani S, Lexcel-

lent C (2009) Multiaxial shape memory effect and super-

elasticity. Strain 45(1):7784

26. Grabe C, Bruhns O (2009) Path dependence and multi-

axial behavior of a polycrystalline NiTi alloy within the

pseudoelastic and pseudoplastic temperature regimes. Int

J Plast 25(3):513545

27. Birman V (1997) Review of mechanics of shape memory

alloy structures. Appl Mech Rev 50(11):629645

28. Paiva A, Savi M (2006) An overview of constitutive models

for shape memory alloys. Math Probl Eng 2006:130

29. Khandelwal A, Buravalla V (2009) Models for shape

memory alloy behavior: an overview of modeling approa-

ches. Int J Struct Changes Solids 1(1):111148

30. Tokuda M, Ye M, Takakura M, Sittner P (1999) Thermo-

mechanical behavior of shape memory alloy under complex

loading conditions. Int J Plast 15(2):223239

31. Bouvet C, Calloch S, Lexcellent C (2004) A phenomeno-

logical model for pseudoelasticity of shape memory alloys

under multiaxial proportional and nonproportional loadings.

Eur J Mech-A/Solids 23(1):3761

32. Thiebaud F, Collet M, Foltete E, Lexcellent C (2007)

Implementation of a multi-axial pseudoelastic model to

Meccanica

123

predict the dynamic behavior of shape memory alloys.

Smart Mater Struct 16:935

33. Pan H, Thamburaja P, Chau F (2007) Multi-axial behavior

of shape-memory alloys undergoing martensitic reorienta-

tion and detwinning. Int J Plast 23(4):711732

34. Arghavani J, Auricchio F, Naghdabadi R, Reali A, Soh-

rabpour S (2010) A 3-D phenomenological constitutive

model for shape memory alloys under multiaxial loadings.

Int J Plast 26(7):976991

35. Saleeb A, Padula S II, Kumar A (2011) A multi-axial,

multimechanism based constitutive model for the compre-

hensive representation of the evolutionary response of

SMAs under general thermomechanical loading conditions.

Int J Plast 27(5):655687

36. Raniecki B, Lexcellent C, Tanaka K (1992) Thermody-

namic models of pseudoelastic behaviour of shape memory

alloys. Arch Mech 44:261284

37. Khachaturian A (1983) Theory of structural transformations

in solids. Wiley, New York

38. Melnik R, Roberts A, Thomas K (1999) Modelling

dynamics of shape-memory-alloys via computer algebra.

Proc SPIE Math Control Smart Struct 3667:290301

39. Melnik R, Roberts A, Thomas KA (2000) Computing

dynamics of copper-based SMA via center manifold

reduction models. Comput Mat Sci 18:255268

40. Artemev A, Jin Y, Khachaturyan A (2001) Three-dimen-

sional phase field model of proper martensitic transforma-

tion. Acta Mater 49(7):11651177

41. Chen L (2002) Phase field models for microstructure evo-

lution. Annu Rev Mater Res 32:113140

42. Levitas V, Preston D (2002) Three-dimensional Landau

theory for multivariant stress-induced martensitic phase

transformations. II. Multivariant phase transformations and

stress space analysis. Phys Rev B 66(134206):115

43. Ahluwalia R, Lookman T, Saxena A (2006) Dynamic strain

loading of cubic to tetragonal martensites. Acta Materialia

54:21092120

44. Wang L, Melnik R (2007) Finite volume analysis of non-

linear thermo-mechanical dynamics of shape memory

alloys. Heat Mass Transf 43(6):535546

45. Bouville M, Ahluwalia R (2008) Microstructure and

mechanical properties of constrained shape memory alloy

nanograins and nanowires. Acta Mater 56(14):35583567

46. Daghia F, Fabrizio M, Grandi D (2010) A non isothermal

GinzburgLandau model for phase transitions in shape

memory alloys. Meccanica 45:797807

47. Dhote R, Fabrizio M, Melnik R, Zu J (2013) Hysteresis

phenomena in shape memory alloys by non-isothermal

GinzburgLandau models. Commun Nonlinear Sci Numer

Simul 18:25492561

48. Idesman A, Cho J, Levitas V (2008) Finite element mod-

eling of dynamics of martensitic phase transitions. Appl

Phys Lett 93(4):043102

49. Melnik R, Roberts A, Thomas KA (2002) Phase transitions in

shape memory alloys with hyperbolic heat conduction and

differential-algebraic models. Comput Mech 29(1):1626

50. Melnik R, Roberts A (2003) Modelling nonlinear dynamics

of shape-memory-alloys with approximate models of cou-

pled thermoelasticity. Z Angew Math Mech 83(2):93104

51. Mahapatra D, Melnik R (2006) Finite element analysis of

phase transformation dynamics in shape memory alloys

with a consistent LandauGinzburg free energy model.

Mech Adv Mater Struct 13:443455

52. Wang L, Melnik R (2010) Low dimensional approximations

to ferroelastic dynamics and hysteretic behavior due to

phase transformations. J Appl Mech 77:031015

53. Dhote R, Melnik R, Zu J (2012) Dynamic thermo-

mechanical coupling and size effects in finite shape memory

alloy nanostructures. Comput Mat Sci 63:105117

54. Wang L, Melnik R (2007) Thermo-mechanical wave

propagation in shape memory alloy rod with phase trans-

formations. Mech Adv Mater Struct 14(8):665676

55. Melnik R, Wang L (2009) International conference on

computational methods for coupled problems in science and

engineering coupled problems 2009, CIMNE, Barcelona

pp. 14.

56. Dhote RP, Melnik RVN, Zu JW (2011) Dynamic thermo-

mechanical properties of shape memory alloy nanowires upon

multi-axial loading. ASME conference on smart materials,

adaptive structures and intelligent systems pp. 411417

57. Dhote R, Gomez H, Melnik R, Zu J. 3D coupled thermo-

mechanical phase-field modeling of shape memory alloy

dynamics via isogeometric analysis (submitted for evalua-

tion, available as arXiv:1403.5612)

58. Dhote R, Gomez H, Melnik R, Zu J. Shape memory alloy

nanostructures with coupled dynamic thermo-mechanical

effects, 2014, (available as arXiv:1403.6133)

59. Falk F (1980) Model free energy, mechanics, and thermo-

dynamics of shape memory alloys. Acta Metall 28(12):

17731780

60. Carstensen C (1996) On the computational of crystalline

microstructure. Acta Numer 5:191256

61. Rabe K, Ahn C, Triscone J (2007) Physics of ferroelectrics:

a modern perspective. Springer, Berlin

62. Clayton JD, Knap J (2011) A phase field model of defor-

mation twinning: nonlinear theory and numerical simula-

tions. Phys D 240(9):841858

63. Hildebrand F, Miehe C (2012) A phase field model for the

formation and evolution of martensitic laminate micro-

structure at finite strains. Philos Mag 92(34):42504290

64. Levin VA, Levitas VI, Zingerman KM, Freiman EI (2013)

Phase-field simulation of stress-induced martensitic phase

transformations at large strains. Int J Solids Struct 50(19):

29142928

65. Phillips R (2001) Crystals, defects and microstructures: mod-

eling across scales. Cambridge University Press, Cambridge

66. Clayton JD (2011) Nonlinear mechanics of crystals, vol

177. Springer, Dordrecht

67. Waitz T, Antretter T, Fischer F, Simha N, Karnthaler H

(2007) Size effects on the martensitic phase transformation

of NiTi nanograins. Acta Mater 55(2):419444

68. Gadaj S, Nowacki W, Pieczyska E (2002) Temperature

evolution in deformed shape memory alloy. Infrared Phys

Technol 43(35):151155

69. Pieczyska E, Gadaj S, Nowacki W, Tobushi H (2006)

Phase-transformation fronts evolution for stress-and strain-

controlled tension tests in TiNi shape memory alloy. Exp

Mech 46(4):531542

70. Pieczyska EA, Tobushi H (2010) Temperature evolution in

shape memory alloy during loading in various conditions.

10th international conference on quantitative infrared

thermography, pp. 16.

Meccanica

123

71. Ricci A, Ricciardi A (2010) A new finite element approach

for studying the effect of surface stress on microstructures.

Sens Actuators A 159:141148

72. Comsol Multi-Physics Modeling and Simulation Software

(2012). URL http://www.comsol.com. Accessed May 2013

73. Park K, Banerjee P (2002) Two-and three-dimensional

transient thermoelastic analysis by BEM via particular

integrals. Int J Solids Struct 39(10):28712892

74. Wang L, Melnik R (2006) Differential-algebraic approach

to coupled problems of dynamic thermoelasticity. Appl

Math Mech 27(9):11851196

75. Sapriel J (1975) Domain-wall orientations in ferroelastics.

Phys Rev B 12(11):5128

76. Yasuda H, Komoto N, Ueda M, Umakoshi Y (2002)

Microstructure control for developing FePd ferromag-

netic shape memory alloys. Sci Technol Adv Mater 3(2):

165169

77. Ma Y, Setzer A, Gerlach JW, Frost F, Esquinazi P, Mayr SG

(2012) Freestanding single crystalline FePd ferromagnetic

shape memory membranesrole of mechanical and mag-

netic constraints across the martensite transition. Adv Funct

Mater 22(12):25292534

78. Liu Y (2001) Detwinning process and its anisotropy in

shape memory alloys. Smart materials and MEMS, Inter-

national Society for Optics and Photonics, pp. 8293.

79. Rejzner J, Lexcellent C, Raniecki B (2002) Pseudoelastic

behaviour of shape memory alloy beams under pure bend-

ing: experiments and modelling. Int J Mech Sci 44(4):

665686

80. Reedlunn B, Churchill CB, Nelson EE, Shaw JA, Daly SH

(2014) Tension, compression, and bending of superelastic

shape memory alloy tubes. J Mech Phys Solids 63:506537

81. Dhote R, Gomez H, Melnik R, Zu J (2013) Isogeometric

analysis of coupled thermo-mechanical phase-field models

for shape memory alloys using distributed computing. Proc

Comput Sci 18:10681076

Meccanica

123

http://www.comsol.com

Dynamic multi-axial behavior of shape memory alloy nanowires with coupled thermo-mechanical phase-field modelsAbstractIntroductionSMA dynamicsNumerical simulationsMicrostructure evolutionMulti-axial loadingNanowire with twinned microstructure as an initial conditionNanowire with austenite microstructure as an initial condition

ConclusionsAcknowledgmentsReferences

Recommended